The Science and Engineering of Materials, 4 th ed Donald R. Askeland – Pradeep P. Phulé Chapter 7 – Strain Hardening and Annealing
Objectives of Chapter 7 <ul><li>To learn how the strength of metals and alloys is influenced by mechanical processing and heat treatments. </li></ul><ul><li>To learn how to enhance the strength of metals and alloys using cold working. </li></ul><ul><li>To learn how to enhance ductility using annealing heat treatment. </li></ul>
Chapter Outline <ul><li>7.1 Relationship of Cold Working to the Stress-Strain Curve </li></ul><ul><li>7.2 Strain-Hardening Mechanisms </li></ul><ul><li>7.3 Properties versus Percent Cold Work </li></ul><ul><li>7.4 Microstructure, Texture Strengthening, and Residual Stresses </li></ul><ul><li>7.5 Characteristics of Cold Working </li></ul><ul><li>7.6 The Three Stages of Annealing </li></ul><ul><li>7.7 Control of Annealing </li></ul><ul><li>7.8 Annealing and Materials Processing </li></ul><ul><li>7.9 Hot Working </li></ul><ul><li>7.10 Superplastic Forming (SPF) </li></ul>
<ul><li>Flow stress </li></ul><ul><li>Strain hardening </li></ul><ul><li>Strain hardening exponent ( n ) </li></ul><ul><li>Strain-rate sensitivity ( m ) </li></ul><ul><li>Bauschinger effect </li></ul>Section 7.1 Relationship of Cold Working to the Stress-Strain Curve
Figure 7.1 Development of strain hardening from the stress-strain diagram
Figure 7.2 Manufacturing processes that make use of cold working as well as hot working. Common metalworking methods
Section 7.2 Strain-Hardening Mechanisms <ul><li>Frank-Read source - A pinned dislocation that, under an applied stress, produces additional dislocations. This mechanism is at least partly responsible for strain hardening. </li></ul><ul><li>Thermoplastics - A class of polymers that consist of large, long spaghetti-like molecules that are intertwined (e.g., polyethylene, nylon, PET, etc.). </li></ul>
Figure 7.5 The Frank-Read source can generate dislocations. (a) A dislocation is pinned at its ends by lattice defects. (b) As the dislocation continues to move, the dislocation bows, eventually bending back on itself. (c) finally the dislocation loop forms, and (d) a new dislocation is created. (e) Electron micrograph of a Frank-Read source (330,000). (Adapted from Brittain, J., ‘‘Climb Sources in Beta Prime-NiAl,’’ Metallurgical Transactions, Vol. 6A, April 1975.)
Example 7.1 Cold Working a Copper Plate A 1-cm-thick copper plate is cold-reduced to 0.50 cm, and later further reduced to 0.16 cm. Determine the total percent cold work and the tensile strength of the 0.16-cm plate. (See Figure 7.8.)
Example 7.2 Design of a Cold Working Process Design a manufacturing process to produce a 0.1-cm-thick copper plate having at least 65,000 psi tensile strength, 60,000 psi yield strength, and 5% elongation. Example 7.2 SOLUTION To produce the plate, a cold-rolling process would be appropriate. The original thickness of the copper plate prior to rolling can be calculated from Equation 7-4, assuming that the width of the plate does not change. Because there is a range of allowable cold work—between 40% and 45%—there is a range of initial plate thicknesses:
Example 7.2 SOLUTION (Continued) To produce the 0.1-cm copper plate, we begin with a 0.167- to 0.182-cm copper plate in the softest possible condition, then cold roll the plate 40% to 45% to achieve the 0.1 cm thickness.
Figure 7.9 The fibrous grain structure of a low carbon steel produced by cold working: (a) 10% cold work, (b) 30% cold work, (c) 60% cold work, and (d) 90% cold work (250). (Source: From ASM Handbook Vol. 9, Metallography and Microstructure, (1985) ASM International, Materials Park, OH 44073. Used with permission.)
Example 7.3 Design of a Stamping Process One method for producing fans for cooling automotive and truck engines is to stamp the blades from cold-rolled steel sheet, then attach the blades to a “spider’’ that holds the blades in the proper position. A number of fan blades, all produced at the same time, have failed by the initiation and propagation of a fatigue crack transverse to the axis of the blade (Figure 7.11). All other fan blades perform satisfactorily. Provide an explanation for the failure of the blades and redesign the manufacturing process to prevent these failures.
<ul><li>Example 7.3 SOLUTION </li></ul><ul><li>The wrong type of steel may have been selected. </li></ul><ul><li>The dies used to stamp the blades from the sheet may be worn. </li></ul><ul><li>The clearance between the parts of the dies may be incorrect, producing defects that initiate fatigue failure. </li></ul><ul><li>The failures could also be related to the anisotropic behavior of the steel sheet caused by rolling. </li></ul>
Example 7.4 Design of a Fatigue-Resistant Shaft Your company has produced several thousand shafts that have a fatigue strength of 20,000 psi. The shafts are subjected to high-bending loads during rotation. Your sales engineers report that the first few shafts placed into service failed in a short period of time by fatigue. Design a process by which the remaining shafts can be salvaged by improving their fatigue properties.
<ul><li>Example 7.4 SOLUTION </li></ul><ul><li>Increasing the strength at the surface improves the fatigue life of the shaft – carburizing </li></ul><ul><li>Cold working the shaft </li></ul><ul><li>Shot peen the shaft </li></ul>
Section 7.6 The Three Stages of Annealing <ul><li>Recovery - A low-temperature annealing heat treatment designed to eliminate residual stresses introduced during deformation without reducing the strength of the cold-worked material. </li></ul><ul><li>Recrystallization - A medium-temperature annealing heat treatment designed to eliminate all of the effects of the strain hardening produced during cold working. </li></ul><ul><li>Grain growth - Movement of grain boundaries by diffusion in order to reduce the amount of grain boundary area. </li></ul>
Figure 7.16 Photomicrographs showing the effect of annealing temperature on grain size in brass. Twin boundaries can also be observed in the structures. (a) Annealed at 400 o C, (b) annealed at 650 o C, and (c) annealed at 800 o C (75). (Adapted from Brick, R. and Phillips, A., The Structure and Properties of Alloys, 1949: McGraw-Hill.)
Section 7.7 Control of Annealing <ul><li>Warm working - A term used to indicate the processing of metallic materials in a temperature range that is between those that define cold and hot working (usually a temperature between 0.3 to 0.6 of melting temperature in K). </li></ul>
Section 7.8 Annealing and Materials Processing <ul><li>Heat-affected zone (HAZ) - The volume of material adjacent to a weld that is heated during the welding process above some critical temperature at which a change in the structure, such as grain growth or recrystallization, occurs. </li></ul>
Example 7.6 Design of a Process to Produce Copper Strip We wish to produce a 0.1-cm-thick, 6-cm-wide copper strip having at least 60,000 psi yield strength and at least 5% elongation. We are able to purchase 6-cm-wide strip only in thicknesses of 5 cm. Design a process to produce the product we need.
Example 7.6 SOLUTION In Example 7-2, we found that the required properties can be obtained with a cold work of 40 to 45%. Therefore, the starting thickness must be between 0.167 cm and 0.182 cm, and this starting material must be as soft as possible— that is, in the annealed condition. Since we are able to purchase only 5-cm thick stock, we must reduce the thickness of the 5-cm strip to between 0.167 and 0.182 cm, then anneal the strip prior to final cold working. But can we successfully cold work from 5 cm to 0.182 cm? Based on Figure 7.7, a maximum of about 90% cold work is permitted. Therefore, we must do a series of cold work and anneal cycles.
Section 7.9 Hot Working <ul><li>Lack of Strengthening </li></ul><ul><li>Elimination of Imperfections </li></ul><ul><li>Anisotropic Behavior </li></ul><ul><li>Surface Finish and Dimensional Accuracy </li></ul>
Example 7.7 Design of a Process to Produce a Copper Strip We want to produce a 0.1-cm-thick, 6-cm-wide copper strip having at least 60,000 psi yield strength and at least 5% elongation. We are able to purchase 6-cm-wide strip only in thicknesses of 5 cm. Design a process to produce the product we need, but in fewer steps than were required in Example 7.6.
Example 7.7 SOLUTION In Example 7.6, we relied on a series of cold work-anneal cycles to obtain the required thickness. We could reduce the steps by hot rolling to the required intermediate thickness: Thus our design might be: 1. Hot work the 5-cm strip 96.4% to the intermediate thickness of 0.182 cm. 2. Cold work 45% from 0.182 cm to the final dimension of 0.1 cm. This design gives the correct dimensions and properties.
Section 7.10 Superplastic Forming (SPF) <ul><li>Superplasticity - The ability of a metallic or ceramic material to deform uniformly by an exceptionally large amount. </li></ul><ul><li>Strain rate - The rate at which a material is deformed. </li></ul>